of 15 /15
Semiconductor Physics Problems 2016 Page and ﬁgure numbers refer to Semiconductor Devices – Physics and Technology, 3rd edition, by SM Sze and M-K Lee 1. The purest semiconductor crystals it is possible to fabricate have about 1 impurity per 10 12 host atoms. Consider Si and answer the following questions: (a) What is the lowest possible concentration of impurities that we can have in a sample? (b) Is it possible for Si to behave as an intrinsic semiconductor at room temperature? E C E 0 1 F(E) E V E A A B C D E F 2. Consider ﬁgures A-F above. (a) Which of the ﬁgures (A-F) best represents a p-type extrinsic semiconductor where all dopants are ionized? (b) Which ﬁgure represents the highest n (concentration of electrons in the conduction band)? 3. Consider two samples: an n-type sample of silicon which has a uniform doping density N D = 10 16 cm -3 of arsenic, and a p-type silicon sample which has N A = 10 15 cm -3 of boron. Determine the following: (a) Consider the n-type material. Find the temperature at which half the impurity atoms are ionized. Assume that all mobile electrons originate from the dopant impurities. (b) For each material, ﬁnd the temperature at which the intrinsic concentration n i ex- ceeds the impurity density by a factor of 10. (c) Assume full ionization of impurities. Find the equilibrium minority-carrier concent- rations in each material at 300 K. (d) Find the Fermi level referred to the valence band edge E V in each material at 300 K. Find also the Fermi level if both types of impurities are present in the same sample (compensation doping) 1
• Author

tranthien
• Category

## Documents

• view

282

4

Embed Size (px)

### Transcript of Semiconductor Physics Problems 2016 - Solid State Physics · Semiconductor Physics Problems 2016...

Semiconductor Physics Problems 2016Page and figure numbers refer to Semiconductor Devices – Physics and Technology, 3rd edition,by SM Sze and M-K Lee

1. The purest semiconductor crystals it is possible to fabricate have about 1 impurity per1012 host atoms. Consider Si and answer the following questions:

(a) What is the lowest possible concentration of impurities that we can have in a sample?

(b) Is it possible for Si to behave as an intrinsic semiconductor at room temperature?

EC

E

0 1 F(E)

EVEA

A B C D E F

2. Consider figures A-F above.

(a) Which of the figures (A-F) best represents a p-type extrinsic semiconductor whereall dopants are ionized?

(b) Which figure represents the highest n (concentration of electrons in the conductionband)?

3. Consider two samples: an n-type sample of silicon which has a uniform doping densityND = 1016 cm−3 of arsenic, and a p-type silicon sample which has NA = 1015 cm−3 ofboron. Determine the following:

(a) Consider the n-type material. Find the temperature at which half the impurity atomsare ionized. Assume that all mobile electrons originate from the dopant impurities.

(b) For each material, find the temperature at which the intrinsic concentration ni ex-ceeds the impurity density by a factor of 10.

(c) Assume full ionization of impurities. Find the equilibrium minority-carrier concent-rations in each material at 300 K.

(d) Find the Fermi level referred to the valence band edgeEV in each material at 300 K.Find also the Fermi level if both types of impurities are present in the same sample(compensation doping)

1

4. (a) Compare the figure above to figure 25 on page 39 in Sze (page 43 in 2nd edition).They essentially show the same kind of data. What is the difference between howdata is plotted? Why do you think we prefer the representation above?

(b) From the figure above, determine the ionization energy of the donor atoms used todope the Si sample.

5. Consider the Fermi level for a boron-doped Si sample with an impurity concentration of1016 cm−3 at 300 K. What fraction of the impurity atoms are ionized? Could we just saythat all of them are ionized?

Hint: select a value for the concentration of ionized acceptors, which also gives you theconcentration of holes. Use this to calculate EF . Use this to evaluate the percentageof ionized acceptors from the Fermi distribution, which you can use to evaluate the EF

again. If necessary, iterate a few times until consistent.

6. For p in a sample where NA > ND we find p as

p =1

2

[NA −ND +

√(NA −ND)2 + 4n2

i

]For what doping levels (see below) can we estimate that p = NA − ND? Use ni =9.65 · 109cm−3 and ni = 2 · 1013 cm−3 for Si and Ge, respectively. All dopings in cm−3.

(a) NA = 1 · 1014 and ND = 1 · 1012, Si sample

(b) NA = 1 · 1014 and ND = 9 · 1013, Si sample

2

(c) NA = 1 · 1014 and ND = 1 · 1012, Ge sample

(d) NA = 1 · 1014 and ND = 9 · 1013, Ge sample

7. Consider a compensated (contains both donor and acceptor impurity atoms in the sameregion) n-type Si sample at T = 300 K, with a conductivity of σ = 16(Ωcm)−1 and anacceptor doping concentration of 1017 cm−3. Determine the donor concentration. Assumecomplete ionization and an electron mobility of µn = 1500 cm2/Vs. ni = 9.65·109 cm−3.

8. HAND-IN Consider a Si sample doped with 1.0 · 1014 cm−3 of phosphorous atoms,8.5 · 1012 cm−3 of arsenic atoms and 1.12 · 1013 cm−3 of boron atoms. Assume that theimpurities are completely ionized and the mobilities are µn = 1500 cm2/Vs, µp = 500cm2/Vs, independent of impurity concentrations. ni = 9.65 · 109 cm−3 in Si at 300 K.

(a) Find the resistivity for the sample.

(b) Find the Fermi level in the sample.

9. Consider a Si sample with a high n-type doping of 5 · 1018 cm−3. Calculate the positionof the Fermi level. Compare the distance from the conduction band edge to kT . Is yourresult for the Fermi level credible?

10. Consider scattering in an n-type semiconductor sample by studying fig 2 on page 46 inSze (p 50 in 2nd edition). Which of the following statements are true?

(a) If doping level is increased a factor 10, conductivity is also increased a factor 10

(b) At high T , lattice/phonon scattering dominates

(c) At room temperature, the scattering time due to lattice scattering is longer than thatdue to impurity scattering in lightly doped samples

(d) If we could remove all impurities, the low T scattering time would increase

11. Compute the average thermal velocity (speed) for holes in a Si sample at room tempe-rature. Next assume that we apply a voltage of 1 mV over a 0.2 mm long section of thesemiconductor. What is the drift velocity? The hole mobility is 400 cm2/Vs.

12. Calculate the electron and hole concentration under steady-state illumination in n-typesilicon with excess generation rate GL = 1016 cm−3s−1, ND = 1015 cm−3 and τp =10µs.

13. HAND-IN Assume that an n-type semiconductor is uniformly illuminated, producing auniform excess generation rate G. Show that in steady state the change in semiconductorconductivity is given by ∆σ = q(µn + µp)τpG.

3

xL0

EC

EF

Ei

EV

14. The energy band diagram for a semiconductor is shown in the figure above. This may forinstance represent the variation of potential along the radius of a n-type semiconductornanowire with the Fermi level pinned close to the valence band edge at the nanowiresurface by surface states.

Sketch the general form of

(a) n and p versus x,

(b) the electrostatic potential Ψ as a function of x,

(c) the electric field as a function of x,

(d) Jn and Jp versus x.

NA2 = 5∙1015 cm-3ND1 = 1017 cm-3

NA1 = 5∙1015 cm-3

region 1 region 2

15. Consider a Si pn-junction with impurity concentrations as indicated in the figure above.Compute

(a) The minority carrier concentration in region 1

(b) The minority carrier concentration in region 2

In order to compute the built-in potential Vbi,

Vbi =kT

qlnX1X2

n2i

which of the following suggestions for X1 and X2 would you use?

(a) X1 = ND1 and X2 = NA2

(b) X1 = ND1 −NA2 and X2 = NA2

(c) X1 = ND1 −NA1 and X2 = NA2

(d) X1 = ND1 and X2 = NA1

4

16. Consider an ideal silicon pn abrupt junction with NA = 1017 cm−3 and ND = 1015

cm−3. Assume that all impurities are completely ionized.

(a) One approach to find the built-in voltage/potential is to consider the p- and n-part ofthe junction separately. Vbi can then be found as the difference between the Fermi-levelEFn on the n-side and the Fermi levelEFp on the p-side, as qVbi = EFn−EFp.Convince yourself that this gives an equation corresponding to equation 12 on page85 in Sze (p. 91 in 2nd edition).

(b) Calculate Vbi at T = 300, 350, 400, 450 and 500 K and plot Vbi vs T .

(c) Try to give a physical explanation for the trend observed in b). Hint: Maybe you canbase your reasoning on the procedure in part a).

(d) Find the depletion layer width and the maximum field at zero bias for T = 300 K.

-2 -1

1 2

1.0·1016

0.5·1016

ND -- NA ((cm-3

)

xx ((µm)

-1015

17. HAND-IN

(a) Find and sketch the charge density, the built-in electric field and the potential for asilicon p-i-n junction with the doping profile shown in the figure above. (”i” repre-sents a very lightly doped or nearly intrinsic region.)

(b) Calculate Vbi and the length of each depletion region at thermal equilibrium.

(c) Compare the maximum field in the pin junction to the maximum field in a pn jun-ction that contains no lightly doped intermediate region, but has the same dopantconcentrations as in part (a) in the other regions.

(d) Make a sketch indicating how the built-in electrical field in the junction changeswhen a reverse bias is applied.

5

-3 -2 -1 1

0.8 V

11.5·1026

11.0·1026

00.5 ·1026

0 VVa ((volts)

Cj2

-2)

18. HAND-IN The depletion layer capacitance CD (denoted Cj in the plot above) of a Si pnjunction diode with area 10−5 cm2 is measured. A plot of (1/C2

D) vs. the applied voltageVa is shown in the figure above.

(a) If the diode is considered as a one-sided step junction, where the p-side is heavilydoped, find the doping level on the n-side.

(b) Sketch (qualitatively) the doping density on the n-side of the p+n junction. Calculatethe location of the point (distance from the actual junction) on the n-side at whichthe dopant density changes, and include this point in your sketch. Indicate how thedopant density changes at this point – does it increase or decrease compared to thevalue you found in a)?

RL=100 kΩ

VR=10 VVF=5 V

19. HAND-IN In an ideal p+n silicon diode with ND = 1015 cm−3 and NA = 1018 cm−3

the hole lifetime is 1 µs and their mobility 450 cm2/Vs. The area of the diode is 0.1mm2. (“Ideal” implies that effects within the space-charge region are negligible and thatminority carriers flow only by diffusion mechanisms in the charge neutral regions.)

(a) Determine the current in the diode when reverse biased. This is accompliced byflipping the switch in the figure above (as indicated).

(b) Estimate the stored minority carrier charge when the diode is forward biased in thecircuit above.

(c) Turning the switch will reverse bias the diode. Determine the change in fix chargein the depletion region on the n side when the diode is switched from forward toreverse bias.

6

20. Consider an ideal, long-base, silicon abrupt pn-junction diode with uniform cross sectionand constant doping on either side of the junction. The diode is made from 1 Ω-cm p-typeand 0.2 Ω-cm n-type materials in which the minority-carrier lifetimes are τn = 10−6 sand τp = 10−8 s, respectively. You may find figure 7 on page 51 of Sze (p 55 in 2ndedition) and fig 3 on page 47 (p 51) useful.

(a) What is the value of the built-in voltage (built-in potential)?

(b) Calculate the density of the minority carriers at the edge of the space-charge regionwhen the applied voltage is 0,589 V (which is 23kT/q).

(c) Sketch the majority- and minority-carrier currents as functions of distance from thejunction on both sides of the junction, under the applied bias voltage of part b.

(d) Calculate the location(s) of the plane or planes at which the minority-carrier andmajority-carrier currents are equal in magnitude for the applied bias of part b.

21. (a) For forward voltages between 0 and 0.6 V, plot (on a logarithmic scale) the diffusioncurrent in a Si p+n-junction. In the same plot, include also the recombination current(eq 59 on page 105, p 110 in 2nd edition). You may assume ND = 1015 cm−3, µp= 500 cm2/Vs and Dp= 10 cm2/s and a life-time τp = τ = 1µs. For the purpose ofcalculating the built-in potential you can use for instance NA = 1017 cm−3.

(b) Finally, plot the sum of the two current contributions, also in the same plot. Try toidentify regions with ideality factor 1 or 2 (see page 106 (p 112 in 2nd edition) fordefinition of ideality factor)

7

22. A Si npn transistor has impurity concentrations of 5 · 1018 cm−3, 2 · 1017 cm−3 and 1016

cm−3 in the emitter, base and collector, respectively. The p-type base width is 1.0 µm,and the device cross-sectional area is 0.2 mm2. When the emitter-base junction is forwardbiased to 0.5 V and the base-collector junction is reverse biased to 5 V, calculate

(a) the neutral base width and

(b) the minority carrier concentration in the base at the edge of the emitter-base junctiondepletion region.

23. HAND-IN The figure above depicts a pnp bipolar transistor and all the currents which weconsider in it.

(a) Draw an equivalent figure, still for a pnp-transistor, where you instead of currentsdraw electron and hole flows.

(b) Draw an equivalent figure for a npn transistor, where you draw currents. Label thecurrents in a way appropriate to the npn-transistor.Make nice big figures, so that everything is clearly visible.

8

24. HAND-IN Consider Eq. 14 on p. 130 in Sze (2nd edition; see Eq. (14) p. 138) for thedistribution of minority carriers in the base of an pnp bipolar transistor in the active mo-de (EB junction forward biased and BC junction reverse biased). The equation can bereorganized to read:

pn(x)− pn0 = (pn(0)− pn0)sinh(W−xLp

)

sinh(WLp

)+ (pn(W )− pn0)

sinh( xLp

)

sinh(WLp

)

where x = 0 and x = W are the edges of the neutral base.

(a) For a Si pnp-transistor, plot pn(x)/pn0 as a function of x/W for different values ofW . In your plot, include the following neutral base widths W :

W/Lp = 100, 10, 5, 2, 1, 0.5, 0.1 and 0.01.

All graphs should be in the same plot (this is why the x-axis should be normalizedto x/W ). You can assume VEB = 0.5 V, VCB = −1 V, NB = 1016 cm−3 andLp = 10−4 cm (the minority carrier diffusion length in the base).

(b) Using the plots in a), evaluate the ratio ICp/IEp for the different base widths W .Hint – the currents can be obtained by estimating the gradients of the minority carrierdistributions.Make a graph where you plot the ratios ICp/IEp for different W vs W . Since Wvaries over four orders of magnitude, you need to use a logarithmic scale on the x-axis. Verify your results by comparing your ratios to the theoretical ratio ICp/IEp =1/ cosh(W/Lp) .

(c) Write a short text (150 words is sufficient) describing how your plots are significantto our discussion of bipolar transistors.

25. HAND-IN Consider a Si npn transistor. The area of the device is 1.2 · 10−4 cm2. Inabsence of applied bias, the neutral base width is 4 ·10−4 cm. For the transistor we furtherhave:NE = 3.9 · 1017 cm−3 NB = 1.6 · 1016 cm−3 NC = 2 · 1014 cm−3

LE = 22.8 · 10−4 cm LB = 46.9 · 10−4 cm LC = 39.5·10−4 cmDE = 5.18 cm2/s DB = 22 cm2/s DC = 15.6 cm2/s

(a) For a forward bias of VEB = 0.6 V on the emitter-base junction, calculate IEn

and IEp (it is OK to use the expressions for current for short bases, that is, whenW/Ln < 1). Also calculate the emitter efficiency γ . You don’t need to care aboutthe change in W due to biasing.

(b) What is the emitter efficiency if the emitter is doped to the same level as the base,that is, NE = NB = 1.6 · 1016 cm−3?

9

26. For the transistor of problem 25, consider the emitter-base junction open-circuited and thebase-collector junction reverse biased by -1 V. Find VEB and ICBO (that is the current inthe base-collector junction when the emitter current is zero).

The neutral base width in the absence of applied biases is stated in problem 25. Here, thereis a reverse bias applied to the base-collector junction. Since the collector is lightly dopedthe depletion region at the base-collector junction will expand mainly into the collector,and thus the base width will not be significantly reduced. You can use the value of problem25 as the base width W .

27. Consider the lower image on p 72 of the notes. It shows band diagrams for a pnp-transistorin the four modes of operation. Draw the equivalent images for a npn transistor. By equiva-lent we mean that the axes stay the same, for instance that a positive VEB means VE > VB .This will forward bias the EB-junction in a pnp-transistor, but what is the effect in a npn-transistor?

vin

vout

VCC = +12 V

RC

RB C

EB

28. The transistor in the circuit shown in the figure above has a common-emitter current gainβ = 100.

The resistors in the circuit are RC = 1 kΩ and RB = 20 kΩ. Assume VEB = 0.6 V forthe forward biased EB junction.

Determine vout for vin = 1 V and 2 V.

29. For an ideal MOS with a n-type semiconductor under inversion, plot

(a) the space charge distribution

(b) the electric field

(c) the potential

10

30. We want to find the threshold voltage VT for inversion in a p-type Si MOS in terms ofmaterial constants, such as dielectric constants, and in terms of parameters that we control,such as doping level. The voltage VT is split between the oxide and the semiconductor, sothat VT = ΨS + V0.

The band bending (in inversion) is primarily given by the depleted region in the semicon-ductor. Here, we have a space charge density ρ = −qNA for 0 ≤ x ≤ W (see figure).From that we find the potential

Ψ(x) =qNA

2εs(x−W )2 = Ψs(1−

x

W)2

where Ψs = qNA2εs

W 2

(a) Deep in the p-type semiconductor pp0 = NA. Start from p = nie(Ei−EF )/kT and

show that ΨB = (kT/q) ln(NA/ni)

(b) In strong inversion the electron concentration at the surface ns ≥ NA. Starting fromns = nie

(EF−Eis)/kT , where Eis is the intrinsic Fermi level at the surface, showthat EF − Eis = ΨB when ns = NA. The potential at the surface thus has to beΨS = 2ΨB for inversion.

(c) Now consider the voltage drop Vo over the oxide. From electrostatics, we found thatVo = d · Qm

εox= d · |Qs|

εox. At the onset of strong inversion, |Qs| can be approximated

by |Qsc| where Qsc is the charge from the depleted acceptors. In inversion, Qsc =−qNAWm.Show that the depletion region widthW can be written in terms of the surface poten-tial asW =

√2εsΨsqNA

(see beginning of problem) and that, consequently, in inversion,

Wm =√

2εs2ΨBqNA

.

(d) Now we put our results together. Show that the threshold voltage

VT = Ψs(inv) + Vo = 2kTq ln NA

ni+√

ε2oxkT ln NA

ni

11

E F E F

qψB

d

E i

ψ

xW

0

-V FB

31. HAND-IN For the Si MOS structure above, the work function in the metal is smallerthan that of the semiconductor by 1V (we disregard any oxide charges). The potential inthe metal relative to in the semiconductor, |VFB|, is the sum of a potential drop over theoxide and a potential drop over the depleted region of the semiconductor. Consider thesemiconductor to be grounded. The oxide thickness d = 10 nm, the oxide permittivity isεox = 3.9ε0 and NA = 1017cm−3.

(a) What is the value of the surface potential?

(b) What is the electric field in the oxide?

(c) What are the values of electron and hole concentrations at the surface of the semi-conductor?

32. Consider a MOS device on a p-type substrate (NA = 1017cm−3) with 20 nm of gateoxide. The gate is made of polycrystalline n+-Si. When used as a gate electrode, the n+-Si is very heavily doped and essentially the Fermi level coincides with the conductionband edge.

(a) Find the work function difference between the polycrystalline Si gate and the p-typeSi semiconductor.

(b) Find VT .

(c) Make a sketch of the C − V curve measured at high frequencies. In your sketch,label (roughly) VT and VFB .

(d) Calculate Cmin and Cmax (still for high frequency).

12

33. A Si MOSFET has the following dimensions and characteristic parameters: L = 1 µm,Z = 1 µm, NA = 1017 cm−3, µn = 800 cm2/Vs and the Si oxide thickness is 20 nm.The semiconductor work function is 3.8 V and the gate work function is 4 V.

(a) Sketch the band diagram at thermal equilibrium and at threshold condition Ψs =2ΨB . What is the threshold voltage?

(b) Calculate the drain current for VG = 2.2 V and VD = 0.3 V.

(c) Calculate the drain current for VG = 2.5 V and VD = 0.3 V.

34. A n-channel MOSFET is made on p-type silicon with NA = 4 · 1015 cm−3.

(a) Determine the threshold voltage under the assumption that the oxide (rel. dielectricconstant 3.9) is free of charge and that difference in work functions may be neglec-ted. The gate oxide is 100 nm thick.

(b) Sketch the drain current vs the gate voltage for the MOSFET of part a) if drain andgate are connected and source and substrate are grounded. Can the threshold voltagebe determined from the characteristic?

35. Threshold voltage control is an important concept. In devices such as CMOS (Compli-mentary MOS – one PMOS and one NMOS acting together as for instance an inverter)and generally in circuits, we may want to tailor the threshold voltage. There are severalapproaches to this.

Consider a N-MOS with gate and semiconductor parameters as in problem 32.

(a) Is the N-MOS conducting at VG = 0?

(b) Find the change in doping necessary to change VT by −0.5 V. Here, we assume thatthe doping is changed to a large depth in the semiconductor, not only just below theoxide.

(c) Find the change in oxide thickness needed to accomplish the same shift of VT as inb)

13

36. HAND-IN A MOSFET has a threshold voltage of VT = 0.5 V, a subthreshold swing of100 mV/decade, and a drain current of 0.1 mA at VT .

(a) What is the subthreshold leakage current at VG = 0V? (Hint: think about what thesubthreshold swing really means.)

(b) In the MOSFET lab, you measured drain current as a function of gate and drainvoltage. The figure shows the drain current at a fixed VD > VDsat) for varying VGfor one of the devices in the lab. Was it the NMOS or the PMOS and what is thesubthreshold swing?

−3.8 −3.6 −3.4 −3.2 −3 −2.8 −2.6 −2.410

−8

10−7

10−6

10−5

10−4

10−3

10−2

10−1

gate voltage / V

drai

n cu

rren

t /A

(ab

solu

te v

alue

)

14

37. HAND-IN

(a) Find the barrier height and the donor concentration of the W- GaAs Schottky barriershown in the capacitance plot above left. Note that the plot show two different data-sets - make sure you read values of the correct y-axis.

(b) Compare the barrier height with that obtained from the saturation current densityshown in the current plot above right, assuming that A∗ = 4 A/(cm-K)2.

38. Compare a Schottky diode fabricated on n-GaAs and a p+n diode (also GaAs). The reversesaturation currents are Is = 5 · 10−9 A and I0 = 10−13 A for the Schottky diode and thepn-junction, respectively. What voltage is required for each device in order to have 0.5mA pass through it?

39. This problem concerns the discussion in the Sze e-book (which is linked from the coursehomepage). The relevant pages are 139-144. See also notes.

(a) In figure 6 on page 143 we notice that c2 = 0.27 is relevant for Si. This numberthus tells us something about the nature of the population of surface states in Si.Assuming an interface layer with thickness δ = 5Å and permittivity εi = ε0 and asemiconductor doping of ND = 1018cm−3, calculate the density of interface statesDit. (check your answer on page 142).

(b) If the Fermi level does not coincide with the neutral level, there will be a net chargeat the interface. By how much can the Fermi level deviate from the neutral levelin order for the interface charge Qss to not become greater than the semiconductorchargeQsc (from ionized dopants)? Here you will have to obtain a value for Vbi(Ψbi)at some point. Either you can just assume some reasonable value, or use fig. 5 onpage 140 in the book. Ψbi = Eg − qφn − qφ0, if we make the approximation thatEF coincides with φ0 (not completely true, but not far from the truth either, it willdo as an estimate). φ0 is calculated at the bottom of p. 142.

15